1 ALD Film Characterization Rachel Brown 5/13/14 Objective The following set of tests was performed to determine the characteristics of films created by the Atomic Layer system and how they varied with the operation temperature. The films tested were aluminum oxide, hafnium oxide, and zinc oxide. The use of different recipes was also tested to determine the temperature ranges best suited to a recipe. Procedure Each wafer was run for 8 cycles at its respective temperature and recipe. Four measurements were made on each sample: deposition rate, index of refraction, stress, and roughness measurements: The Gaertner Ellipsometer was used to take measurements of the wafer film thickness before and after ALD processing by measuring five points on each wafer to determine the film thickness. measurements: The Gaertner Ellipsometer was used to take five measurements on the surface of each wafer giving an average index of refraction value. measurements: Each wafer was scanned three times in the Test-1 before and after ALD processing to measure the stress induced by the film. It was found that the extra film deposited on the outer edge of the backside of each wafer can significantly affect stress measurements. To eliminate the effects of this factor, we removed the extra film on each wafer before taking stress measurements. This was accomplished using two different methods: For aluminum and zinc films: After taking the deposition rate and index of refraction measurements, the front side of the wafer was coated with S13 photoresist. Wafers were soft-baked and then immersed in a BOE bath for about 3 minutes or until the backside film was removed. Once the photoresist was removed with solvents, the second stress measurement was taken. For hafnium films: The BOE solution is ineffective in removing this film. Instead, the Oxford Etcher recipe N etch al was used for about 1 minutes with the same coating of photoresist as described above and the wafer placed face down in the machine. Then the photoresist was removed and the stress measurement was taken. Roughness measurements: Roughness measurements were taken by the Atomic Force Microscope. A 1 µm and a 1 µm image were taken of each sample. The Rms and Ra of each image were taken by the AFM roughness analysis. In the graphs displayed in this report, a measurement labeled 1 refers to the 1 µm image and a measurement labeled 2 refers to the 1 µm image of each sample.
2 Results Summary of Results Temp per 1 cycles) Roughness per 1 cycles) Hf2O3 Roughness Temp per 1 cycles) Roughness
3 (Angstroms per 1 cycles) Low Temperature Recipes Temp per 1 cycles) per 1 cycles) s HfO
4 : HfO
5 (Mpa) (Mpa) (Mpa) : HfO
6 Roughness (nm) Roughness (nm) Roughness: Aluminum Oxide: Aluminum Oxide Film Roughness Rms 1 Ra 1 Rms 2 Ra (A measurement labeled 1 refers to the 1 µm image and a measurement labeled 2 refers to the 1 µm image of each sample.) Hafnium Oxide: 7 6 Hafnium Oxide Film Roughness Rms 1 Ra 1 Rms 2 Ra
7 Roughness (nm) Zinc Oxide: 6 Zinc Oxide Film Roughness Rms 1 Ra 1 Rms 2 Ra